Comparative study of electrolyte additives using electrochemical impedance spectroscopy on symmetric...
Embed Size (px)
Transcript of Comparative study of electrolyte additives using electrochemical impedance spectroscopy on symmetric...
housie UcMedtronic Energy and Component Center, 6700 Shingl
c cells itive eleive elecOBX, Limbic e
Article history:Received 9 September 2013
The effect of various electrolyte additives and additive combinations added to a 1 M LiPF6 EC:EMCelectrolyte on the positive and negative electrodes surface of 1 year old wound LiCoO /graphite cells and
. All rights reserved.
trolyte can in some cases lead to extended lifetime as shown byBroussely et al.  and to better rate performances [2,3].
Even if these additives are nowwidely used in the Li-ion batteryindustry, the details of how they work are poorly understood. Forexample, VC was thought to be a good additive for the formation of
the negative elec-[4,5.6]. It is nowact of VC is at the
of these additivesantial amounts of
resources to their study [7e10]. For example, Burns et al. [3,5] usedhigh precision coulometry, automated storage and electrochemicalimpedance spectroscopy (EIS) to evaluate the effect of additives onthe cycling performances of commercial wound LiCoO2/graphiteand Li[Ni0.4Mn0.4Co0.2]O2/graphite cells. Amongst other things,they showed that VC reduces the rate of parasitic reactions at thepositive electrode, that TMOBX leads to greater parasitic reaction atthe positive electrode but lowers the impedance, that the mix ofTMOBX and VC leads to a good balance between reduced rate of
* Corresponding author. Dept. of Chemistry, Dalhousie University, Halifax, NovaScotia, Canada B3H4R2.
Contents lists available at ScienceDirect
Journal of Pow
Journal of Power Sources 251 (2014) 187e194E-mail address: firstname.lastname@example.org (J.R. Dahn). 2013 Elsevier B.V
Li ion batteries have high gravimetric and volumetric energydensities, which make them suitable for transport applications.However parasitic reactions between the electrolyte and the elec-trodes limit their lifetime. The addition of additives to the elec-
an efcient solid electrolyte interface (SEI) attrode, which has been recently questionedbelieved by some that the major benecial imppositive electrode.
In an effort to better understand the roleseveral research groups have dedicated substElectrolyte additivesImpedance spectroscopyPrecision coulometrySolid electrolyte interphase
in Li[Ni0.4Mn0.4Co0.2]O2/graphite wound cells. Higher charge voltage led to higher positive electrodeimpedance, with the exception of 2%VC 2% FEC, and 2% LiTFSI. In some cases, some additives whenmixed with another controlled the formation of the SEI at one electrode, and shared the formation of theSEI at one electrode when mixed with a different additive.Received in revised form7 November 2013Accepted 15 November 2013Available online 28 November 2013
Li[Ni0.4Mn0.4Co0.2])O2/graphite cells was studied using electrochemical impedance spectroscopy (EIS) onsymmetric cells. The additives tested were: vinylene carbonate (VC), trimethoxyboroxine (TMOBX),uoroethylene carbonate (FEC), lithium bis(triuoromethanesulfonyl)imide (LiTFSI), and H2O alone or incombination. In general, compared to control electrolyte, the additives tested reduced the impedance ofthe positive electrode and increased the impedance of the negative electrode with the exception of LiTFSIh i g h l i g h t s
Impedance spectroscopy on symmetri Almost all additives increase the nega Almost all additives decrease the posit Additives studied include VC, FEC, TM The impact of these additives on coulo
a r t i c l e i n f o0378-7753/$ e see front matter 2013 Elsevier B.V.http://dx.doi.org/10.1016/j.jpowsour.2013.11.054e Creek Parkway, Brooklyn Center, MN, USA
s used to determine which electrodes additives inuence most.ctrode impedance.trode impedance.TFSI and water and their combinations.fciency was also measured.
a b s t r a c taDept. of Chemistry, Dalhousie University, HalibDept. of Physics and Atmospheric Science, Dal niversity, Halifax, Nova Scotia, Canada B3H3J5Gaurav Jain , S. Trussler , J.R. Dahnfax, Nova Scotia, Canada B3H4R2Comparative study of electrolyte additivimpedance spectroscopy on symmetric
R. Petibon a, N.N. Sinha b, J.C. Burns b, C.P. Aiken b, Hc b a,b,*
journal homepage: www.eAll rights reserved.using electrochemicallls
Ye c, Collette M. VanElzen c,
vier .com/locate/ jpowsour
at 10 C and 30 C in that order. All EIS spectra were taken using aBioLogic VMP3 equipped with 2 EIS boards. Many EIS spectra werecollected over the course of these experiments and in order toautomate the process somewhat, the output of one VMP3 EIS boardwas connected to a Keithley 705 scanner and the output of theother to a Keithley 706 scanner. Each scanner housed two Keithley705310-channel high current scanner cards. In-house softwarewasdesigned and written so that each scanner could connect up to 16cells sequentially to have their EIS spectra measured automaticallyovernight. All impedance spectra were collected at constant tem-perature by housing the cells in temperature-controlled boxes at10.0 and 30.0 0.2 C.
3. Results and discussion
As shown in Ref.  the impedance of the positive symmetriccells grows over time, whereas the impedance of the full cells andnegative symmetric cells are stable. This indicates the existence ofan interaction between the positive and negative electrodes in thefull cell that somehow prevents the impedance of the positiveelectrode from growing. It also suggests the existence of an auto-
2% FEC (Novolyte) Yes Yes Yes2% LiTFSI (3 M, 99.9%) Yes Yes Yes
werparasitic reactions at the positive electrode and reduced impedanceleading to good overall cell performances (rate capability and ca-pacity retention). However, the effect of these additives on theimpedance of the positive and negative electrode was notdetermined.
In order to easily detect the effect of an additive at the positiveelectrode and negative electrode separately, a method based onelectrochemical impedance spectroscopy of symmetric cellsdeveloped by Chen et al.  was recently introduced . Thistechnique allows one to extract the effect of an additive on thecharge transfer resistance (Rct) of the positive electrode and nega-tive electrode. Rct of each electrode can be related to the nature ofthe SEI on the positive and negative electrode. Comparing the Rct ofboth electrodes allows the effect of an additive on the positive andnegative electrode to be detected (if the products of the reactionsare insoluble). This technique proved to be very useful in studyingthe effect of VC and TMOBX on both electrodes of wound LiCoO2/graphite cells. Petibon et al. showed that VC greatly reduced Rct ofthe positive electrode at both 1 wt% and 2 wt%, VC did not stronglyeffect Rct of the negative electrode at 1 wt%, but greatly increasedRct of the negative electrode at 2 wt%. They also showed thatTMOBX does not strongly affect the negative electrode impedancebut greatly reduces Rct of the positive electrode when 0.3 wt% ofTMOBX is used. Finally, Petibon et al. showed that when 2 wt% VCand 0.3 wt% TMOBX were introduced, the effect of VC at thenegative electrode and the effect of TMOBX at the positive elec-trode were maintained.
In this paper similar studies to those of Petibon et al.  arereported for a relatively large set of additives studied over a periodof more than two years. The additives, 2 wt% FEC, 2 wt% LiTFSI,100 ppm H2O and several pairs of additives in addition to 2 wt% VCand 0.3 wt% TMOBX have been studied to determine their effect onthe Rct of the positive and negative electrodes of wound Li[Ni0.4Mn0.4Co0.2]/graphite cells (called NMC cells), and two groupsof LiCoO2/graphite cells charged to different cut-off voltages (calledLV-LCO and HV-LCO cells). It is believed that this work will be ofinterest to scientists trying to improve the lifetime of Li-ion cells.
Wound prismatic LiCoO2/graphite and Li[Ni0.4Mn0.4Co0.2]O2/graphite cells with 1 M LiPF6, EC:EMC (3:7 by weight) were used inthis study. The cells studied contained approximately 1.5 g ofelectrolyte per gram of negative active material. Table 1 lists theadditives tested inwhich cell chemistries. Some combinations werenot tested due to unavailability of cells.
Fig. 1 shows the history of the cells used in this study. The cellswere rst subjected to an automated storage test . This testconsists of two dischargeecharge cycles between the lower andupper voltage cut-off, followed by an open circuit storage step of500 h at the top of charge. The two dischargeecharge cycles and theopen circuit voltage steps are then repeated one more time. Thelower and upper voltage cut-offs of the NMC cells were 3.3 V and4.225 V, respectively. Two groups of LiCoO2/graphite cells wereused. The lower and upper voltage cut-offs of the rst group, calledLV-LCO cells, were 3.4 V and 4.075 V, respectively. The lower andupper voltage cut-offs of the second group, called HV-LCO cells,were 3.4 V and 4.175 V, respectively. All cells contained the samegraphite negative electrode and their negative to positive activematerial ratio was balanced according to their voltage cut-off. Theratios of the active mass of the positive electrode and the activemass of the negative electrode for the LV-LCO cells, HV-LCO, andNMC cells were 1.6, 1.4, and 1.2 respectively. After the automatedstorage test the cells were then put away for approximately one
R. Petibon et al. / Journal of Po188year at an open circuit voltage around 3.9 V at room temperature(19 Ce22 C). The cells were then cycled for a short period (one fullcycle) and stopped at an open circuit voltage of 3.775 V corre-sponding to approximately 50% state of charge. The electro-chemical impedance spectra of the cells were then taken at 10 C,20 C, 30 C, and 40 C. Then the cells were taken insi